NEGATIVE REFRACTIVE INDEX BEHAVIOR THROUGH MAGNETO-ELECTRIC COUPLING IN SPLIT RING RES-ONATORS

Z. Djeffal, H. Talleb, D. Lautru, and V. Fouad Hanna

UPMC Univ Paris 06

UR 2, L2E, 4 place Jussieu, F-75005, Paris, France

Abstract—An investigation on the possibility of obtaining a negative refractive index behavior in split ring resonators (SRRs) through magneto-electric coupling is presented. We have performed rigorous electromagnetic simulations using a full-wave 3D simulator, and the obtained results have been verified by our experimental realizations and measurements. The results confirm that the increase of magneto-electric gyrotropic activity inside a bi-anistropic medium can lead to the establishment of backward-wave propagation.

1. INTRODUCTION

The counterintuitive phenomena exhibited by metamaterials, such as the negative refraction and backward-wave propagation, attract many researchers all over the world, especially those who are working on realizing different structures presenting these phenomena in the microwave and optical domains such as mushrooms [1, 2] or photonic crystals [3]. So far, there have been very few successfully realized engineering applications making use of materials that can exhibit backward-wave propagation phenomenon. Most of them use planar microwave circuits [4] behaving as High-Impedance Surfaces (HIS). Nevertheless, experimental investigations on an edge of a prism structure composed of split ring resonators (SRRs) and metallic wires have demonstrated the presence of negative refraction phenomenon. However, these experimental investigations suffer from the presence of ohmic and magnetic losses due to electromagnetic interactions between both SRRs and metallic wires arrays [5].

*Received 8 February 2011, Accepted 11 March 2011, Scheduled 30 March 2011*

In this paper, we confirm the role that the magneto-electric coupling plays in the left-handed behavior of bianisotropic materials as emphasized in previous works in other situations, e.g., it was explained that it is possible to establish of backward-wave propagation in Faraday chiral medium [6, 7] or in simply chiral medium [8–11]. This interpretation can be understood from the fact that a backward-wave can be produced when both of permeability, and permittivity is quite small at the working frequencies or smaller than the magneto-electrique parameter.

In this paper, a rigorous electromagnetic simulation of a periodic and bianisotropic SRRs medium [12, 13] illuminated by a plane-wave is performed. Our results demonstrate the presence of a backward wave propagation associated to gyrotropic phenomenon without a dichroism effect, results that confirm the existence of magnetoelectric coupling. This gyrotropic phenomenon, illustrated by the rotation of electric and magnetic fields for a plane wave propagating in the medium, is caused by a Faraday effect since a magnetic field is spontaneously induced along the direction of propagation of the plane-wave. To confirm this result, a measurement set-up is established using an edge of a prism formed of SRRs medium. The measured negative refraction behavior using the classic deviation angle of rotation shows a good concordance with the simulation results.

2. PROPAGATION IN BIANISOTROPIC MEDIUM

Consider a gyrotropic reciprocal bianisotropic medium whose response to an electromagnetic field is characterized by the following constitutive relations [12, 14, 15]:

*D* = ¯¯*²E*+ ¯¯*χH* (1)

*B* = *−χ*¯¯*TE*+ ¯¯*µH* (2)

where*D, B, E, H* denote respectively, the electric displacement vector,
the magnetic induction field, the electric field vector and the magnetic
field. Theses relations can be written in the following harmonic
standard form (the time-dependence is suppressed here):

*E*(*r*) = *E*0exp(*ik*0*k*˜*ur*ˆ ) (3)

*H*(*r*) = *H*0exp(*ik*0˜*kur*ˆ ) (4)

ˆ

*u,*˜*k*and *k*_{0} =*ω√²*_{0}*µ*_{0} denote the unit vector, the relative wave vector
(˜*k* *∈* C), and the free space wave number respectively. *²*0 and *µ*0 are
the permittivity and permeability in free space, respectively. Here, a
uniaxial system is chosen considering that the optical axis is along the
ˆ

¯¯

*χ,*¯¯*²* and ¯¯*µ* denote, according to [15, 6], the coupling dyadic
parameter expressing magnetoelectric effects, permittivity and
permeability constitutive tensors, respectively:

¯¯

*χ* = [*χxyx*ˆ*y*ˆ+*χyxy*ˆ*x*ˆ] (5)

¯¯

*²* = *²*0

h

*²⊥I*¯¯*−i²gz*ˆ*×I*¯¯+ (*²z−²⊥*)ˆ*zz*ˆ

i

(6) ¯¯

*µ* = *µ*0

h

*µ _{⊥}I*¯¯

*−iµgz*ˆ

*×I*¯¯+ (

*µz−µ⊥*)ˆ

*zz*ˆ

i

(7)

*χ _{xy}, χ_{yx}, ²_{g}* and

*µ*are the gyrotropic parameters due to the gyrotropic properties of a composite medium.

_{g}*²*and

_{⊥}*µ*are the permittivity and the permeability in the perpendicular plan to the propagation axis and

_{⊥}¯¯

*I* is the identity matrix.

The system can be reduced to a 2 dimensions one since the wave
vector *k* is parallel to the ˆ*z* direction and both of Dz and Bz are
zero. Using a regular procedure in the k-D-B vector coordinate system
like that used in [16], we obtain the following quadratic polynomial
equation:

*u*4*−*(2*v*+*χ*2* _{xy}* +

*χ*2

*)*

_{yx}*u*2+ (

*v*+

*χ*2

*)(*

_{xy}*v*+

*χ*2

*) =*

_{yx}*b*2 (8) where

*u*=

*=*

_{ω}k, v*²*0

*µ*0(

*²⊥µ⊥*+

*²gµg*) and

*b*=

*²*0

*µ*0(

*²⊥µg*+

*²gµ⊥*).

In the case where *χ _{xy}* =

*−χ*=

_{yx}*−jK*, where

*K*measures the magnetoelectric coupling [15], the solution can be written as:

*ua±* = *±*

q

*²*0*µ*0(*²⊥*+*²g*)(*µ⊥*+*µg*)*−K*2 (9)
*ub±* = *±*

q

*²*0*µ*0(*²⊥−²g*)(*µ⊥−µg*)*−K*2 (10)

by putting *²±*= (*²⊥±²g*) and *µ±*= (*µ⊥±µg*), the solutions yield:

*k*=*±ω*p*²*0*µ*0*²±µ±−K*2 (11)

This solution concords with that given in [15, 12] but it takes
also into consideration the effect of gyrotropy. Let us now, study
the case for which *k* = _{2}*ω _{c}*(

*²±*+

*µ±*), namely the case for which the material parameters satisfy the condition

*K*=

_{2}

*√²*

_{0}

*µ*

_{0}(

*µ*). It can be seen that a backward-wave propagation becomes possible when Re(

_{±}−²_{±}*²±*+

*µ±*)

*<*0, i.e., when the following relation is satisfied:

*−*(*²g*+*µg*)*>*(*²⊥*+*µ⊥*) (12)

3. ELECTROMAGNETIC SIMULATION VALIDATION

Here, we examine the dense copper SRR medium represented in Fig. 1
for which the dimensions of a unit cell are given. The lattice periods
along, *x, y*, and *z* axis are 18 mm, 16.5 mm, and 18 mm, respectively
and the employed substrate is the Epoxy (*² _{r}*= 4

*.*4) with a thickness of 1.5 mm. We restrict our study to the case of a plane wave propagating along the

*z*axis when the electric field and magnetic field are applied along the

*x*axis and the

*y*axis, respectively.

Rigorous electromagnetic simulations performed using the
full-wave 3D CST Microfull-wave Studio software have shown a
backward-wave phenomenon behavior between 9.3–10 GHz (see Fig. 2). To
demonstrate this phenomenon, a prism, composed of the same SRRs
shown above and having an apex angle A of 45*◦*_{, has been illuminated}
by a horn antenna working at 10 GHz. Fig. 3 shows a cross sectional
view of the near field patterns while Fig. 4 shows a maximum deviation

Figure 1. The studied SRRs structure.

Figure 2. Top view of the SRRs structure excited by a plane wave at 9.8 GHz.

angle D of the steering beam equals *−*55*◦* _{in the far field zone. The}
refractive index can be calculated from Equation (13) according the
formulation given in [18]. Thus, we obtain an effective index of*−*0*.*23.

*n*= sin ((*D*+*A*)*/*2)

sin (*A/*2) (13)
To better understand the causality of this phenomenon, some
magnetic and electric probes have been placed inside and along the
studied structure. Fig. 5 shows a cross sectional view inside the
medium in which we can notice the presence of a gyrotropic effect
involving two elliptically polarized electric and magnetic fields.

This gyotropic effect, expressed by the gyrotropic parameters

*K*, *²g* and *µg*, is caused by a Faraday effect since a quasi-static

effective magnetic field Hz is found to oscillate around a mean value of 1.1 mA/V. In fact, each rings cell behaves as magnetic and electric

E (V/m)

Figure 4. Far field radiation pattern in cartesian coordinates at 10 GHz.

dipole particles where the permeability and permittivity can be quite small in the working frequency band around resonance. It is important to emphasize that normally the Faraday effect is a nonreciprocal effect since it is due to the application of an external magnetic field in the direction in propagation of the system, i.e., involving a variance of the results when the transmitter and receiver are interchanged. However, in our case, this effect is reciprocal since the same Hz field is spontaneously induced according to the employed direction of propagation.

4. EXPERIMENTAL CONFIRMATION

To verify these principal simulation results, an experimental setup
operating in the X band was established like that described in [19].
It enables to determine the angular position of a microwave beam
generated from a network analyzer and passes across a SRR prism
medium having an apex angle of 45*◦*_{. The SRR prism has the same}
dimensions of the above simulated prism. As illustrated in Fig. 6, the
microwave beam was generated by a horn antenna placed at a short
distance from the prism. This setup enables to reduce the angular
spread of the incident beam caused by diffraction and also to maximize
the received power. A mobile horn antenna controlled by a stepping
motor was used to capture the microwave beam and to determine the
refractive angle corresponding to its angular position. Fig. 7 shows
the experimental results for the electrical field intensity at 10 GHz
normalized with respect to the maximum intensity received without
the prism at *θ* = 0*◦* _{(i.e., when the transmitting antenna is placed}
directly in front of the receiving antenna without any obstruction). It
can be seen that there are different levels for the received field intensity
according to the position of the receiving antenna. The deviation angle

-90 -80 -70 -60 -50 -40 -30 -20 -10 0 0 0.01 0.02 0.03 0.04 0.05 0.06

Theta / Degree

Enorm

0.07

Figure 7. Variation of the nor-malized received electrical field in-tensity at 10 GHz as a function of the angular displacement of the mobile antenna.

-90 -80 -70 -60 -50 -40 -30 -20 -10 0

0 0.01 0.02 0.03 0.04 0.05 0.06

Theta / Degree

Enorm

*f *=10 GHZ
* f *=10.5 GHZ

Figure 8. Variation of the nor-malized received electrical field in-tensity at 10 GHz and 10.5 GHz as a function of the angular displace-ment of the mobile antenna when an array of ten units of SRRs has been added.

corresponding to the maximum measured electrical field intensity is

*D*=*−θ*=*−*70*◦*_{, which means that the value of the refractive index}* _{n}*
equals

*−*0

*.*56 according (13).

In order to confirm these experimental results and also to reduce
the influence of diffraction phenomenon, an array of ten units of SRRs
was added to the studied prism. The experimental results show a
negative refraction between 9.5 GHz to 10.5 GHz. Fig. 8 shows the
variation of the electrical field intensity at 10 GHz and 10.5 GHz as
a function of the angular displacement of the mobile antenna. One
can notice that the deviation angle at both 10 GHz and 10.5 GHz,
corresponds to a negative refraction, since the angle of the maximum
measured electrical field intensity at both 10 GHz and 10.5 GHz is*−*62*◦*
and*−*56*◦*_{respectively with a corresponding refractive index (according}
to (13)) *n*=*−*0*.*4 and*n*=*−*0*.*25 respectively. One can also notice a
decrease of the value of the measured maximum received electric field
intensity at 10 GHz due to additional losses introduced by the added
SRR structure.

5. CONCLUSION

the realization of LHMs with negligible ohmic and magnetic losses since it is not recessionary to add metallic wires to obtain a backward propagation. The measurement setup, using an edge of a prism formed of SRRs medium, has enabled us to measure a negative refraction and validated the simulation results. The addition of an array of SRRs structure has confirmed the measured negative refractions. This study has been performed in the microwave domain, and it is evident that a transposition can be extended to other frequency ranges since the scaling principle can be applied.

REFERENCES

1. Sievenpiper, D., L. Zhang, R. F. J. Broas, N. G. Alexopolous, and
E. Yablonovitch, “High-impedance electromagnetic surfaces with
a forbidden frequency band,”*IEEE Trans. on Microwave Theory*
*and Techniques, Vol. 47, No. 11, 2059–2074, November 1999.*
2. Grbic, A. and G. V. Eleftheriades, “Periodic analysis of a

2-D negative refractive indextransmission line structure,” *IEEE*
*Trans. on Antennas and Propagation, Vol. 51, No. 10, 2604–2611,*
October 2003.

3. Srivastava, R., S. Srivastava, and S. P. Ojha, “Negative refraction
by photonic crystal,” *Progress In Electromagnetics Research B,*
Vol. 2, 15–26, 2008.

4. Hrabar, S., “Backward-wave meta-materials — A brief review,”
*17’International Conference on Applied Electromagnetics and*
*Communications, Dubrovnik, Croatia, October 1–3, 2003.*

5. Simovski, C. A. and B. Sauviac, “Role of wave interaction of wire
and split-ring resonators for the losses in a left-handed composite,”
*Phys. Review E, Vol. 70, 046607, 2004.*

6. Mackay, T. G. and A. Lakhtakia, “Plane waves with negative
phase velocity in Faraday chiral mediums,” *Phys. Review E,*
Vol. 69, 026602, 2004.

7. Mackay, T. G. and A. Lakhtakia, “Negative reflection in a Faraday
chiral medium,” *Micro. Opt. Tech. Lett., Vol. 50, No. 5, 1368–*
1371, May 2008.

8. Qiu, C. W., H. Y. Yao, L. W. Li, S. Zouhdi, and T. S. Yeo,
“Routes to left-handed materials by magnetoelectric couplings,”
*Phys. Review B, Vol. 75, 245214, 2007.*

10. Qiu, C. W., H. Y. Yao, S. Zouhdi, L. W. Li, and M. S. Leong, “On
the constitutive relations of G-chiral media and the possibility to
realize negative-index media,” *Micro. Opt. Tech. Lett., Vol. 48,*
No. 12, 2534–2538, December 2006.

11. Taouk, H., “Optical wave propagation in active media:
Gyrotropic-gyrochiral media,” *J. Opt. Soc. Am.* Vol. 14, No. 8,
2006–2012, August 1997.

12. Marques, R., F. Medina, and R. Rafii-El-Idrissi, “Role of
bian-isotropy in negative permeability and left-handed metamaterials,”
*Phys. Review B, Vol. 65, 144440, 2002.*

13. Chen, X., B. Wu, J. A. Kong, and T. M. Grzegorczyk,
“Retrieval of the effective constitutive parameters of bianisotropic
metamaterials,”*Phys. Review E, Vol. 71, 046610, 2005.*

14. Tretyakov, S. A. and A. A. Sochava “Novel uniaxial bianisotropic
materials: Reflection and transmission in planar structures,”
*Progress In Electromagnetics Research, Vol. 9, 157–179, 1994.*
15. Tretyakov, S. A., C. R. Simovski, and M. Hudlicka, “Bianisotropic

route to the realization and matching of backward-wave
metamaterial slabs,”*Phys. Review B, Vol. 75, 153104, 2007.*
16. Kong, J. A.,*Electromagnetic Wave Theory, 1986.*

17. Yang, J., J. Hwang, and T. Timusk, “Left-handed behavior
of split-ring resonators: Optical measurements and numerical
analysis,”*Phys. Review B, Vol. 77, 205114, 2008.*

18. Born, M. and E. Wolf,*Principle of Optics, 7th edition, 1999.*
19. Shelby, R. A., D. R. Smith, and S. Schultz, “Experimental